fabrication of planar semiconductor diodes : an educational laboratory experiment fabrication of...
Post on 11-May-2020
Embed Size (px)
Fabrication of planar semiconductor diodes : an educational laboratory experiment Citation for published version (APA): Heijnen, C. J. H., Jansen, H. A., Olijslagers, J. F. G. J., & Versnel, W. (1981). Fabrication of planar semiconductor diodes : an educational laboratory experiment. (EUT report. E, Fac. of Electrical Engineering; Vol. 81-E-119). Eindhoven: Technische Hogeschool Eindhoven.
Document status and date: Published: 01/01/1981
Document Version: Publisher’s PDF, also known as Version of Record (includes final page, issue and volume numbers)
Please check the document version of this publication:
• A submitted manuscript is the version of the article upon submission and before peer-review. There can be important differences between the submitted version and the official published version of record. People interested in the research are advised to contact the author for the final version of the publication, or visit the DOI to the publisher's website. • The final author version and the galley proof are versions of the publication after peer review. • The final published version features the final layout of the paper including the volume, issue and page numbers. Link to publication
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
• Users may download and print one copy of any publication from the public portal for the purpose of private study or research. • You may not further distribute the material or use it for any profit-making activity or commercial gain • You may freely distribute the URL identifying the publication in the public portal.
If the publication is distributed under the terms of Article 25fa of the Dutch Copyright Act, indicated by the “Taverne” license above, please follow below link for the End User Agreement: www.tue.nl/taverne
Take down policy If you believe that this document breaches copyright please contact us at: firstname.lastname@example.org providing details and we will investigate your claim.
Download date: 11. May. 2020
Fabrication of Planar Semiconductor Diodes,
an educational laboratory experiment
C.J.H. Heijnen, H.A. Jansen,
J.F.G.J. Olijslagers and W. Versnel
Eindhoven University of Technology Research Reports
EINDHOVEN UNIVERSITY OF TECHNOLOGY
Department of Electrical Engineering
Eindhoven The Netherlands
FABRICATION OF PLANAR SEMICONDUCTOR DIODES,
AN EDUCATIONAL LABORATORY EXPERIMENT
EUT Report 81-E-119
2. General survey of the experiment
3. Steps in the fabrication of the device
4. More detailed description of the process steps
5. Diffusion equation and impurity profile
6. Application of masks
7. Possible measurements on the devices
8. Discussions and conclusion
Appendices 1 and 2.
A description is given of a laboratory experiment, in which students themselves manufacture semiconductor diodes and resistors in half a day. The process used is characterized by diffusion of impurities from an oxide layer into silicon and is not critical in this case. The oxide with impurities is formed at a temperature of 35@oC by chemical vapour deposition of silane, oxygen and phosphine.
Heijnen, C.J .H., H.A. Jansen, J .'P.G.J. Olijslagers and W. Versnel FABRICATION OF PLANAR SEMICONDUCTOR DIODES, AN EDUCATIONAL LABORATORY EXPERIMENT. Department of Electrical Engineering, Eindhoven University of Technology, 1981. EUT Report 81-E-119
Address of the authors:
Electronic Devices Group-, Department of Electrical Engineering, Eindhoven University of Technology, P.O. Box 513, 5600 MB EINDHOVEN, The Netherlands
The idea of this experiment is to enable students to make their own
semiconductor devices on which they finally perform a number of measurements.
Many strictly prescribed operations have to be carried out in making a
semiconductor device. This is contrary to the now well-established practice
in student experiments, where the instructions are so formulated that the
students are confronted with a number of problems which they have to solve
themselves. The intention was here to make that part of the experiment in
which no deviations from the instructions are allowed, i.e. the fabrication,
as short as possible. In the experiment described here that takes half a day
(i.e. four hours).(See [1J for a one-year semiconductor technology course).
This has been achieved first by making only simple devices, diodes and
resistors of comparatively large dimensions, and second by using the technique
of diffusion from doped oxide layers [2J obtained by chemical vapour deposition (shortly CVD) instead of the usual technique of gas diffusion [3J.
The fabrication is described in this report. The measurements to be
performed subsequently and that takes two more half days, are only shortly
summarized (section 7), as they have been dealt with extensively elsewhere . In Sections 2 to 6 the experiment is described as presented to the:Students.
A drawing of the CVD reactor is given in appendix I. In appendix 2 the lay-out
and dimensions of the room in which the students do the experiment is shown.
2. GENERAL SURVEY OF THE EXPERIMENT
The original slice of p-type silicon has a diameter of 5.7 cm (2~ inches)
and a thickness of 400 ~m. The specific resistance of the slice is
p = 1.8 - 2.4 ncm. At certain positions n-type regions will be formed by diffusion. The depth
of the n-type diffusion is of the order of 1 ~m. The configuration obtained
is shown in Fig. 1.
0.4 mm p-Si
Fig. I Configuration of sZice with diffu8ed n-region8 in a p-substrate
After all the actions have been performed, the slice is cut along the
broken lines (see Fig. 1), resulting in a large number of diodes and resistors
(more than 4000).
Slice cutting will not be done by the students. They just measure the
electrical behaviour of the diodes and the resistors on the slice itself.
In the next section the steps that lead to a semiconductor device
will be treated summarily, and the separate process steps are described
in more detail in section 4. In Section 5 an introduction is given on
the diffusion equation and on'impurity profiles. In Section 6 we deal
with the applied masks. Several measurements can be carried out on the devjces obtained. They are summed up in Section 7.
3. THE STEPS IN THE FABRICATION OF THE DEVICE
In this section a general description will be given of the steps that
have to be taken to obtain a semiconductor device.
Silicon reacts with oxygen at temperatures above gOOOe [3J. The outer
layer of the slice oxidizes, so that the slice is covered by a layer of 8i0 2
An oxide produced in this way is called a thermal oxide.
The oxide has the following advantages!
1. The oxide layer acts as a protecting mask against penetration of
2. The layer is an insulator. This makes it possible to put conducting
strips on the oxide which make contact with the silicon only at those
places where windows are present in the oxide layer.
3. The crystal lattice of silicon dioxi~e matches fairly well with the
crystal lattice of silicon. This implies a kind of stabilization of
the silicon surface: foreign atoms can easily attach themselves to
the surface of uncovered silicon.
In order to obtain windows in the oxide a photographic process is used.
The oxide is covered with a thin, uniform layer of photoresist, a light-
sensitive material. By means of a mask, i.e. a photographic (glass) plate
with a black and white pattern for the windows, the photoresist is
partially exposed to light. Polymerization occurs at the exposed regions.
By means of a developer the photoresist at the unexposed regions*) is
removed. Then, the slice is placed in a bath filled with a silicon etch.
The oxide will be etched away only at those regions where the photoresist
layer has been removed (Fig. 2).
In addition to the thermal oxidation process another oxidation process is
applied in the semiconductor technology, viz. by chemical vapour deposition
(CVD). In the latter process the gaseous silicon compound silane SiH 4
At 350°C silane alrea